LMucko/crystallography-open-database huggingface dataset:
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm60, T = 844 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006988
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm60, T = 844 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.4 O3 Ti0.6'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.12187
_cell_length_b                   5.12187
_cell_length_c                   14.0077
_cell_formula_units_Z            6
_cell_volume                     318.240
_database_code_amcsd             0008573
_diffrn_ambient_temperature      1117.15
_exptl_crystal_density_diffrn    4.850
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Fe1.4 Ti.6) O3'
_cod_database_code               9006988
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm60, T = 921 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006989
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm60, T = 921 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.4 O3 Ti0.6'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.12710
_cell_length_b                   5.12710
_cell_length_c                   14.0198
_cell_formula_units_Z            6
_cell_volume                     319.166
_database_code_amcsd             0008574
_diffrn_ambient_temperature      1194.15
_exptl_crystal_density_diffrn    4.836
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Fe1.4 Ti.6) O3'
_cod_database_code               9006989
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm60, T = 999 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006990
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm60, T = 999 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.4 O3 Ti0.6'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.13219
_cell_length_b                   5.13219
_cell_length_c                   14.0326
_cell_formula_units_Z            6
_cell_volume                     320.092
_database_code_amcsd             0008575
_diffrn_ambient_temperature      1272.15
_exptl_crystal_density_diffrn    4.822
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Fe1.4 Ti.6) O3'
_cod_database_code               9006990
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm60, T = 795 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006991
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm60, T = 795 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.4 O3 Ti0.6'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.11880
_cell_length_b                   5.11880
_cell_length_c                   14.0020
_cell_formula_units_Z            6
_cell_volume                     317.729
_database_code_amcsd             0008576
_diffrn_ambient_temperature      1068.15
_exptl_crystal_density_diffrn    4.858
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.4 Ti.6) O3'
_cod_database_code               9006991
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm60, T = 594 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006992
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm60, T = 594 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.4 O3 Ti0.6'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.10615
_cell_length_b                   5.10615
_cell_length_c                   13.9817
_cell_formula_units_Z            6
_cell_volume                     315.702
_database_code_amcsd             0008577
_diffrn_ambient_temperature      867.15
_exptl_crystal_density_diffrn    4.889
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.4 Ti.6) O3'
_cod_database_code               9006992
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm60, T = 392 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006993
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm60, T = 392 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.4 O3 Ti0.6'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.09407
_cell_length_b                   5.09407
_cell_length_c                   13.9592
_cell_formula_units_Z            6
_cell_volume                     313.705
_database_code_amcsd             0008578
_diffrn_ambient_temperature      665.15
_exptl_crystal_density_diffrn    4.920
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.4 Ti.6) O3'
_cod_database_code               9006993
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm60, T = 203 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006994
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm60, T = 203 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.4 O3 Ti0.6'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.08205
_cell_length_b                   5.08205
_cell_length_c                   13.9390
_cell_formula_units_Z            6
_cell_volume                     311.774
_database_code_amcsd             0008579
_diffrn_ambient_temperature      476.15
_exptl_crystal_density_diffrn    4.950
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.4 Ti.6) O3'
_cod_database_code               9006994
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 209 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006995
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 209 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.08175
_cell_length_b                   5.08175
_cell_length_c                   13.9383
_cell_formula_units_Z            6
_cell_volume                     311.722
_database_code_amcsd             0008580
_diffrn_ambient_temperature      482.15
_exptl_crystal_density_diffrn    4.939
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9006995
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 301 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006996
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 301 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.08755
_cell_length_b                   5.08755
_cell_length_c                   13.9485
_cell_formula_units_Z            6
_cell_volume                     312.662
_database_code_amcsd             0008581
_diffrn_ambient_temperature      574.15
_exptl_crystal_density_diffrn    4.924
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9006996
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 398 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006997
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 398 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.09392
_cell_length_b                   5.09392
_cell_length_c                   13.9672
_cell_formula_units_Z            6
_cell_volume                     313.866
_database_code_amcsd             0008582
_diffrn_ambient_temperature      671.15
_exptl_crystal_density_diffrn    4.905
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9006997
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 497 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006998
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 497 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.09968
_cell_length_b                   5.09968
_cell_length_c                   13.9803
_cell_formula_units_Z            6
_cell_volume                     314.871
_database_code_amcsd             0008583
_diffrn_ambient_temperature      770.15
_exptl_crystal_density_diffrn    4.889
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9006998
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 597 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9006999
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 597 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.10668
_cell_length_b                   5.10668
_cell_length_c                   13.9928
_cell_formula_units_Z            6
_cell_volume                     316.019
_database_code_amcsd             0008584
_diffrn_ambient_temperature      870.15
_exptl_crystal_density_diffrn    4.871
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9006999
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 697 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9007000
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 697 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.11451
_cell_length_b                   5.11451
_cell_length_c                   14.0061
_cell_formula_units_Z            6
_cell_volume                     317.290
_database_code_amcsd             0008585
_diffrn_ambient_temperature      970.15
_exptl_crystal_density_diffrn    4.852
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9007000
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 745 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9007001
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 745 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.11897
_cell_length_b                   5.11897
_cell_length_c                   14.0135
_cell_formula_units_Z            6
_cell_volume                     318.011
_database_code_amcsd             0008586
_diffrn_ambient_temperature      1018.15
_exptl_crystal_density_diffrn    4.841
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9007001
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 794 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9007002
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 794 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.12327
_cell_length_b                   5.12327
_cell_length_c                   14.0202
_cell_formula_units_Z            6
_cell_volume                     318.698
_database_code_amcsd             0008587
_diffrn_ambient_temperature      1067.15
_exptl_crystal_density_diffrn    4.830
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9007002
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 818 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9007003
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 818 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.12539
_cell_length_b                   5.12539
_cell_length_c                   14.0237
_cell_formula_units_Z            6
_cell_volume                     319.041
_database_code_amcsd             0008588
_diffrn_ambient_temperature      1091.15
_exptl_crystal_density_diffrn    4.825
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9007003
Short- and long-range ordering in the ilmenite-hematite solid solution Sample: ilm65, T = 843 C
Harrison, R. J.; Redfern, S. A. T.; Physics and Chemistry of Minerals 28 (2001) 399–412; doi:10.1007/s002690100167

data_9007004
_publ_section_title
;
 Short- and long-range ordering in the ilmenite-hematite solid solution
 Sample: ilm65, T = 843 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              399
_journal_page_last               412
_journal_paper_doi               10.1007/s002690100167
_journal_volume                  28
_journal_year                    2001
_chemical_formula_sum            'Fe1.35 O3 Ti0.65'
_chemical_name_mineral           Ilmenite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.12732
_cell_length_b                   5.12732
_cell_length_c                   14.0255
_cell_formula_units_Z            6
_cell_volume                     319.323
_database_code_amcsd             0008589
_diffrn_ambient_temperature      1116.15
_exptl_crystal_density_diffrn    4.821
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Fe1.35 Ti.65) O3'
_cod_database_code               9007004